# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_mo_20210521_JZY_SH_1
_database_code_depnum_ccdc_archive 'CCDC 2094409'
loop_
_audit_author_name
_audit_author_address
'Hao Sun'
;Beijing Institute of Technology
China
;
_audit_update_record             
;
2021-07-05 deposited with the CCDC.	2022-05-16 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Co4 H48 K10 O92 P2 W18'
_chemical_formula_weight         5518.34

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/n'
_space_group_name_Hall           '-P 2yn'

_shelx_space_group_comment       
; 
The symmetry employed for this shelxl refinement is uniquely defined 
by the following loop, which should always be used as a source of 
symmetry information in preference to the above space-group names. 
They are only intended as comments. 
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   12.365(6)
_cell_length_b                   21.330(11)
_cell_length_c                   15.827(8)
_cell_angle_alpha                90
_cell_angle_beta                 92.395(15)
_cell_angle_gamma                90
_cell_volume                     4170(4)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    9410
_cell_measurement_theta_min      2.26
_cell_measurement_theta_max      28.26

_exptl_crystal_description       prism
_exptl_crystal_colour            purple
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.394
_exptl_crystal_F_000             4888
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.250
_exptl_crystal_size_mid          0.220
_exptl_crystal_size_min          0.180
_exptl_absorpt_coefficient_mu    26.145
_shelx_estimated_absorpt_T_min   0.059
_shelx_estimated_absorpt_T_max   0.089
_exptl_absorpt_correction_type   Multi-scan
_exptl_absorpt_correction_T_min  0.437
_exptl_absorpt_correction_T_max  0.746
_exptl_absorpt_process_details   sadabs
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            42967
_diffrn_reflns_av_unetI/netI     0.0615
_diffrn_reflns_av_R_equivalents  0.0710
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_k_max       29
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_theta_min         1.603
_diffrn_reflns_theta_max         29.498
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measured_fraction_theta_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             11593
_reflns_number_gt                9578
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
; 
 Reflections were merged by SHELXL according to the crystal 
 class for the calculation of statistics and refinement. 
  
 _reflns_Friedel_fraction is defined as the number of unique 
 Friedel pairs measured divided by the number that would be 
 possible theoretically, ignoring centric projections and 
 systematic absences. 
;

_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick 2008)'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0476P)²+15.9807P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_extinction_coef       0.000440(18)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         11593
_refine_ls_number_parameters     616
_refine_ls_number_restraints     121
_refine_ls_R_factor_all          0.0492
_refine_ls_R_factor_gt           0.0370
_refine_ls_wR_factor_ref         0.0996
_refine_ls_wR_factor_gt          0.0923
_refine_ls_goodness_of_fit_ref   1.020
_refine_ls_restrained_S_all      1.019
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Co1 Co -0.03448(9) 0.55768(5) 0.43439(8) 0.0108(2) Uani 1 1 d . . . . .
Co2 Co -0.21359(10) 0.47665(5) 0.52529(8) 0.0118(2) Uani 1 1 d . . . . .
P1 P 0.06682(16) 0.42457(9) 0.35872(13) 0.0061(4) Uani 1 1 d . . . . .
W1 W 0.01815(3) 0.26084(2) 0.29825(2) 0.01037(8) Uani 1 1 d . . . . .
W2 W -0.06089(3) 0.38999(2) 0.14989(2) 0.01110(8) Uani 1 1 d . . . . .
W3 W 0.23098(3) 0.35413(2) 0.19432(2) 0.01094(8) Uani 1 1 d . . . . .
W4 W 0.13629(3) 0.29717(2) 0.49433(2) 0.01112(8) Uani 1 1 d . . . . .
W5 W -0.13205(3) 0.32953(2) 0.45228(2) 0.00962(8) Uani 1 1 d . . . . .
W6 W -0.20807(3) 0.45909(2) 0.30618(2) 0.01043(8) Uani 1 1 d . . . . .
W7 W -0.01216(3) 0.54421(2) 0.21218(2) 0.01216(8) Uani 1 1 d . . . . .
W8 W 0.27534(3) 0.50807(2) 0.25726(2) 0.01249(8) Uani 1 1 d . . . . .
W9 W 0.34515(3) 0.38957(2) 0.39096(2) 0.01096(8) Uani 1 1 d . . . . .
O1 O -0.0564(5) 0.3148(3) 0.2178(4) 0.0127(12) Uani 1 1 d . . . . .
O2 O 0.0918(5) 0.3797(3) 0.1457(4) 0.0148(13) Uani 1 1 d . . . . .
O3 O 0.1462(5) 0.2909(3) 0.2484(4) 0.0119(12) Uani 1 1 d . . . . .
O4 O 0.0012(5) 0.1887(3) 0.2514(4) 0.0179(14) Uani 1 1 d . . . . .
O5 O -0.1030(6) 0.3624(3) 0.0524(4) 0.0204(15) Uani 1 1 d . . . . .
O6 O 0.2821(6) 0.3127(3) 0.1121(4) 0.0218(15) Uani 1 1 d . . . . .
O7 O 0.1005(5) 0.2407(3) 0.3961(4) 0.0137(13) Uani 1 1 d . . . . .
O8 O -0.1082(5) 0.2669(3) 0.3618(4) 0.0135(13) Uani 1 1 d . . . . .
O9 O -0.1927(5) 0.4094(3) 0.2010(4) 0.0129(12) Uani 1 1 d . . . . .
O10 O -0.0408(5) 0.4757(3) 0.1269(4) 0.0135(12) Uani 1 1 d . . . . .
O11 O 0.2798(5) 0.4355(3) 0.1754(4) 0.0147(13) Uani 1 1 d . . . . .
O12 O 0.3368(5) 0.3422(3) 0.2808(4) 0.0119(12) Uani 1 1 d . . . . .
O13 O -0.0189(5) 0.2843(3) 0.5118(4) 0.0138(13) Uani 1 1 d . . . . .
O14 O -0.1967(5) 0.3792(3) 0.3618(4) 0.0108(12) Uani 1 1 d . . . . .
O15 O -0.1635(5) 0.5263(3) 0.2380(4) 0.0151(13) Uani 1 1 d . . . . .
O16 O 0.1374(5) 0.5248(3) 0.2016(4) 0.0149(13) Uani 1 1 d . . . . .
O17 O 0.3829(5) 0.4571(3) 0.3174(4) 0.0136(13) Uani 1 1 d . . . . .
O18 O 0.2572(5) 0.3231(3) 0.4309(4) 0.0131(12) Uani 1 1 d . . . . .
O19 O 0.1929(6) 0.2416(3) 0.5617(5) 0.0233(16) Uani 1 1 d . . . . .
O20 O -0.2451(5) 0.2976(3) 0.4942(4) 0.0196(14) Uani 1 1 d . . . . .
O21 O -0.3474(5) 0.4694(3) 0.3012(4) 0.0206(15) Uani 1 1 d . . . . .
O22 O -0.0278(6) 0.6085(3) 0.1481(5) 0.0247(16) Uani 1 1 d . . . . .
O23 O 0.3561(6) 0.5622(3) 0.2081(5) 0.0247(16) Uani 1 1 d . . . . .
O24 O 0.4718(5) 0.3638(3) 0.4246(5) 0.0186(14) Uani 1 1 d . . . . .
O25 O 0.0354(5) 0.3584(3) 0.3885(4) 0.0115(12) Uani 1 1 d . U . . .
O26 O -0.0163(5) 0.4450(3) 0.2889(4) 0.0104(12) Uani 1 1 d . U . . .
O27 O 0.1799(5) 0.4207(3) 0.3190(4) 0.0090(11) Uani 1 1 d . U . . .
O28 O 0.0677(5) 0.4704(3) 0.4339(4) 0.0079(11) Uani 1 1 d . U . . .
O29 O 0.1319(5) 0.3669(3) 0.5555(4) 0.0131(12) Uani 1 1 d . U . . .
O30 O -0.1057(5) 0.4001(3) 0.5161(4) 0.0130(12) Uani 1 1 d . U . . .
O31 O -0.1644(5) 0.4991(3) 0.4036(4) 0.0132(13) Uani 1 1 d . U . . .
O32 O 0.0058(5) 0.5770(3) 0.3147(4) 0.0157(13) Uani 1 1 d . U . . .
O33 O 0.2410(5) 0.5460(3) 0.3520(4) 0.0173(14) Uani 1 1 d . . . . .
O34 O 0.3055(5) 0.4436(3) 0.4697(4) 0.0165(13) Uani 1 1 d . . . . .
K1 K -0.27974(19) 0.28659(12) 0.23195(16) 0.0284(5) Uani 1 1 d . . . . .
K2 K -0.3801(3) 0.18130(15) 0.47699(19) 0.0480(8) Uani 1 1 d D . . . .
K3 K 0.338(3) 0.6614(15) 0.358(2) 0.043(5) Uani 0.35(7) 1 d . U P A 1
O40' O 0.087(5) 0.698(2) 0.310(3) 0.045(10) Uani 0.35(7) 1 d . U P A 1
K3' K 0.302(2) 0.6725(7) 0.3426(11) 0.047(3) Uani 0.65(7) 1 d . U P A 2
O40 O 0.035(3) 0.7079(11) 0.3088(14) 0.049(7) Uani 0.65(7) 1 d . U P A 2
K4 K 0.2914(3) 0.62315(17) 0.0539(2) 0.0606(10) Uani 1 1 d . . . . .
K5 K 0.5886(4) 0.57704(18) 0.2147(3) 0.0758(13) Uani 1 1 d . . . . .
O35 O -0.3544(6) 0.4271(4) 0.4957(5) 0.0320(19) Uani 1 1 d . . . . .
O36 O -0.4387(8) 0.2558(5) 0.3413(7) 0.048(2) Uani 1 1 d . . . . .
O37 O -0.4590(7) 0.3692(5) 0.2000(7) 0.051(3) Uani 1 1 d . . . . .
O38 O -0.2497(12) 0.1569(5) 0.2146(8) 0.082(4) Uani 1 1 d . U . . .
O39 O -0.4976(10) 0.2746(5) 0.5591(7) 0.059(3) Uani 1 1 d . . . . .
O41 O 0.5208(7) 0.5557(4) 0.4002(6) 0.039(2) Uani 1 1 d . . . . .
O42 O 0.1900(10) 0.6942(6) 0.1704(10) 0.085(5) Uani 1 1 d . . . . .
O43 O 0.5064(11) 0.6418(6) -0.0134(11) 0.094(5) Uani 1 1 d . . . . .
O44 O 0.1824(16) 0.4938(10) 0.0142(11) 0.048(5) Uani 0.6 1 d . U P . .
O44' O 0.163(2) 0.4635(12) 0.0065(18) 0.039(6) Uani 0.4 1 d . U P . .
O45 O -0.196(2) 0.1439(12) 0.4025(17) 0.111(11) Uani 0.69(4) 1 d . U P . .
O45' O -0.194(3) 0.097(2) 0.442(4) 0.10(2) Uani 0.31(4) 1 d D U P . .
O46 O 0.339(2) 0.5254(14) -0.082(2) 0.097(9) Uani 0.5 1 d . U P . .
O47 O 0.454(3) 0.4983(14) 0.070(2) 0.105(10) Uani 0.5 1 d . U P . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Co1 O29 2.020(6) 3_566 ?
Co1 O32 2.022(7) . ?
Co1 O31 2.077(6) . ?
Co1 O30 2.077(6) 3_566 ?
Co1 O28 2.223(6) 3_566 ?
Co1 O28 2.250(6) . ?
Co2 O33 2.043(7) 3_566 ?
Co2 O34 2.049(7) 3_566 ?
Co2 O35 2.073(7) . ?
Co2 O31 2.099(6) . ?
Co2 O30 2.116(6) . ?
Co2 O28 2.202(6) 3_566 ?
Co2 K3 3.84(3) 3_566 ?
Co2 K3' 3.986(13) 3_566 ?
P1 O28 1.540(6) . ?
P1 O26 1.540(6) . ?
P1 O25 1.544(6) . ?
P1 O27 1.558(6) . ?
W1 O4 1.718(6) . ?
W1 O7 1.868(6) . ?
W1 O8 1.897(6) . ?
W1 O3 1.909(6) . ?
W1 O1 1.923(6) . ?
W1 O25 2.528(6) . ?
W1 K3' 3.723(12) 2_545 ?
W1 K3 3.76(2) 2_545 ?
W1 K1 3.827(3) . ?
W1 K5 4.139(4) 2_545 ?
W2 O5 1.711(7) . ?
W2 O10 1.882(6) . ?
W2 O9 1.895(6) . ?
W2 O2 1.905(6) . ?
W2 O1 1.930(6) . ?
W2 K1 3.764(3) . ?
W2 K2 3.912(4) 4_665 ?
W3 O6 1.715(7) . ?
W3 O11 1.865(6) . ?
W3 O12 1.872(6) . ?
W3 O3 1.930(6) . ?
W3 O2 1.933(6) . ?
W3 K2 3.728(3) 4_665 ?
W3 K3' 3.937(19) 2_545 ?
W4 O19 1.723(7) . ?
W4 O29 1.777(6) . ?
W4 O18 1.916(6) . ?
W4 O13 1.969(6) . ?
W4 O7 2.001(6) . ?
W4 O25 2.427(6) . ?
W4 K4 3.901(4) 2_545 ?
W5 O20 1.713(6) . ?
W5 O30 1.835(6) . ?
W5 O13 1.915(6) . ?
W5 O14 1.929(6) . ?
W5 O8 1.989(6) . ?
W5 O25 2.420(6) . ?
W5 K3' 3.942(14) 3_566 ?
W5 K1 3.975(3) . ?
W5 K3 4.03(2) 3_566 ?
W6 O21 1.736(7) . ?
W6 O31 1.824(6) . ?
W6 O15 1.891(7) . ?
W6 O14 1.919(6) . ?
W6 O9 1.990(6) . ?
W6 O26 2.417(6) . ?
W6 K5 3.800(4) 1_455 ?
W6 K1 3.952(3) . ?
W7 O22 1.713(7) . ?
W7 O32 1.772(6) . ?
W7 O16 1.909(7) . ?
W7 O15 1.969(7) . ?
W7 O10 2.010(6) . ?
W7 O26 2.441(6) . ?
W8 O23 1.733(7) . ?
W8 O33 1.772(7) . ?
W8 O16 1.920(6) . ?
W8 O17 1.937(6) . ?
W8 O11 2.022(6) . ?
W8 O27 2.432(6) . ?
W8 K3 3.70(2) . ?
W8 K3' 3.769(13) . ?
W8 K4 4.059(4) . ?
W9 O24 1.722(6) . ?
W9 O34 1.781(7) . ?
W9 O18 1.911(6) . ?
W9 O17 1.922(7) . ?
W9 O12 2.014(6) . ?
W9 O27 2.392(6) . ?
O1 K1 2.844(7) . ?
O2 K2 3.003(7) 4_665 ?
O3 K3' 2.988(15) 2_545 ?
O3 K3 3.24(4) 2_545 ?
O4 K5 2.691(8) 2_545 ?
O4 K3 2.75(2) 2_545 ?
O4 K3' 2.92(2) 2_545 ?
O5 K4 2.833(8) 3_565 ?
O5 K2 3.187(8) 4_665 ?
O6 K2 2.873(8) 4_665 ?
O6 K3' 3.26(2) 2_545 ?
O7 K4 2.935(7) 2_545 ?
O8 K1 2.921(7) . ?
O9 K1 2.882(7) . ?
O14 K1 3.001(6) . ?
O15 K5 3.257(8) 1_455 ?
O19 K1 2.768(8) 4_666 ?
O19 K4 3.131(8) 2_545 ?
O20 K3' 2.780(15) 3_566 ?
O20 K3 2.80(2) 3_566 ?
O20 K2 2.996(7) . ?
O21 K5 2.772(8) 1_455 ?
O22 K2 2.727(7) 2_455 ?
O23 K4 2.849(8) . ?
O23 K5 2.890(9) . ?
O23 K3 3.19(3) . ?
O23 K3' 3.260(16) . ?
O33 K3 2.74(2) . ?
O33 K3' 2.808(14) . ?
K1 O36 2.751(10) . ?
K1 O38 2.806(12) . ?
K1 O37 2.860(10) . ?
K2 O45 2.72(2) . ?
K2 O36 2.744(11) . ?
K2 O39 2.814(11) . ?
K2 O45' 2.99(4) . ?
K2 O44' 3.17(3) 4_566 ?
K3 O39 2.70(3) 3_566 ?
K3 O35 2.99(4) 3_566 ?
K3 O41 3.24(5) . ?
K3 O40' 3.26(4) . ?
K3' O39 3.03(3) 3_566 ?
K3' O42 3.04(3) . ?
K3' O35 3.37(2) 3_566 ?
K3' O40 3.41(2) . ?
K4 O42 2.732(14) . ?
K4 O43 2.933(15) . ?
K4 O46 3.07(4) . ?
K4 O44 3.12(2) . ?
K4 O47 3.34(3) . ?
K4 K5 4.491(6) . ?
K5 O45 2.73(2) 2 ?
K5 O38 2.817(13) 2 ?
K5 O45' 2.88(5) 2 ?
K5 O41 3.121(11) . ?
K5 O46 3.18(4) 3_665 ?
K5 O47 3.24(4) . ?
O44 O44' 0.70(3) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O29 Co1 O32 94.8(3) 3_566 . ?
O29 Co1 O31 92.3(3) 3_566 . ?
O32 Co1 O31 97.0(3) . . ?
O29 Co1 O30 96.7(3) 3_566 3_566 ?
O32 Co1 O30 91.8(3) . 3_566 ?
O31 Co1 O30 166.9(3) . 3_566 ?
O29 Co1 O28 90.3(2) 3_566 3_566 ?
O32 Co1 O28 174.8(2) . 3_566 ?
O31 Co1 O28 83.5(2) . 3_566 ?
O30 Co1 O28 86.9(2) 3_566 3_566 ?
O29 Co1 O28 174.8(2) 3_566 . ?
O32 Co1 O28 90.3(2) . . ?
O31 Co1 O28 86.0(2) . . ?
O30 Co1 O28 84.3(2) 3_566 . ?
O28 Co1 O28 84.6(2) 3_566 . ?
O33 Co2 O34 92.6(3) 3_566 3_566 ?
O33 Co2 O35 85.6(3) 3_566 . ?
O34 Co2 O35 88.3(3) 3_566 . ?
O33 Co2 O31 172.7(3) 3_566 . ?
O34 Co2 O31 91.6(3) 3_566 . ?
O35 Co2 O31 100.5(3) . . ?
O33 Co2 O30 90.7(3) 3_566 . ?
O34 Co2 O30 174.2(3) 3_566 . ?
O35 Co2 O30 96.7(3) . . ?
O31 Co2 O30 84.6(3) . . ?
O33 Co2 O28 90.5(2) 3_566 3_566 ?
O34 Co2 O28 90.7(2) 3_566 3_566 ?
O35 Co2 O28 175.9(3) . 3_566 ?
O31 Co2 O28 83.5(2) . 3_566 ?
O30 Co2 O28 84.5(2) . 3_566 ?
O33 Co2 K3 43.4(4) 3_566 3_566 ?
O34 Co2 K3 112.6(6) 3_566 3_566 ?
O35 Co2 K3 50.8(7) . 3_566 ?
O31 Co2 K3 139.1(4) . 3_566 ?
O30 Co2 K3 73.0(6) . 3_566 ?
O28 Co2 K3 126.3(6) 3_566 3_566 ?
O33 Co2 K3' 41.6(3) 3_566 3_566 ?
O34 Co2 K3' 118.5(4) 3_566 3_566 ?
O35 Co2 K3' 57.7(5) . 3_566 ?
O31 Co2 K3' 139.5(3) . 3_566 ?
O30 Co2 K3' 67.0(4) . 3_566 ?
O28 Co2 K3' 119.7(4) 3_566 3_566 ?
K3 Co2 K3' 7.7(4) 3_566 3_566 ?
O28 P1 O26 111.0(3) . . ?
O28 P1 O25 109.7(3) . . ?
O26 P1 O25 108.0(3) . . ?
O28 P1 O27 111.6(3) . . ?
O26 P1 O27 108.0(3) . . ?
O25 P1 O27 108.5(3) . . ?
O4 W1 O7 101.8(3) . . ?
O4 W1 O8 101.7(3) . . ?
O7 W1 O8 90.5(3) . . ?
O4 W1 O3 102.2(3) . . ?
O7 W1 O3 89.2(3) . . ?
O8 W1 O3 155.7(3) . . ?
O4 W1 O1 101.8(3) . . ?
O7 W1 O1 156.4(3) . . ?
O8 W1 O1 85.8(3) . . ?
O3 W1 O1 84.8(3) . . ?
O4 W1 O25 170.9(3) . . ?
O7 W1 O25 71.9(2) . . ?
O8 W1 O25 72.3(2) . . ?
O3 W1 O25 84.6(2) . . ?
O1 W1 O25 84.7(2) . . ?
O4 W1 K3' 49.7(5) . 2_545 ?
O7 W1 K3' 93.6(4) . 2_545 ?
O8 W1 K3' 151.3(4) . 2_545 ?
O3 W1 K3' 52.9(4) . 2_545 ?
O1 W1 K3' 100.8(3) . 2_545 ?
O25 W1 K3' 135.8(5) . 2_545 ?
O4 W1 K3 42.5(7) . 2_545 ?
O7 W1 K3 99.1(6) . 2_545 ?
O8 W1 K3 144.0(7) . 2_545 ?
O3 W1 K3 59.6(7) . 2_545 ?
O1 W1 K3 97.5(5) . 2_545 ?
O25 W1 K3 143.6(7) . 2_545 ?
O4 W1 K1 84.9(2) . . ?
O7 W1 K1 138.2(2) . . ?
O8 W1 K1 48.0(2) . . ?
O3 W1 K1 130.08(19) . . ?
O1 W1 K1 45.83(19) . . ?
O25 W1 K1 95.41(14) . . ?
K3' W1 K1 120.0(5) 2_545 . ?
K3 W1 K1 112.2(7) 2_545 . ?
O4 W1 K5 25.4(2) . 2_545 ?
O7 W1 K5 89.2(2) . 2_545 ?
O8 W1 K5 79.82(19) . 2_545 ?
O3 W1 K5 124.46(19) . 2_545 ?
O1 W1 K5 113.03(19) . 2_545 ?
O25 W1 K5 145.75(15) . 2_545 ?
K3 W1 K5 65.9(6) 2_545 2_545 ?
K1 W1 K5 79.69(8) . 2_545 ?
O5 W2 O10 101.4(3) . . ?
O5 W2 O9 103.0(3) . . ?
O10 W2 O9 89.6(3) . . ?
O5 W2 O2 101.1(3) . . ?
O10 W2 O2 88.1(3) . . ?
O9 W2 O2 155.7(3) . . ?
O5 W2 O1 102.5(3) . . ?
O10 W2 O1 156.0(3) . . ?
O9 W2 O1 87.1(3) . . ?
O2 W2 O1 85.3(3) . . ?
O5 W2 K1 85.0(2) . . ?
O10 W2 K1 137.6(2) . . ?
O9 W2 K1 48.51(19) . . ?
O2 W2 K1 132.2(2) . . ?
O1 W2 K1 47.56(19) . . ?
O5 W2 K2 52.9(2) . 4_665 ?
O10 W2 K2 99.1(2) . 4_665 ?
O9 W2 K2 155.50(19) . 4_665 ?
O2 W2 K2 48.3(2) . 4_665 ?
O1 W2 K2 93.60(19) . 4_665 ?
K1 W2 K2 116.97(7) . 4_665 ?
O6 W3 O11 103.0(3) . . ?
O6 W3 O12 102.5(3) . . ?
O11 W3 O12 91.3(3) . . ?
O6 W3 O3 101.5(3) . . ?
O11 W3 O3 155.1(3) . . ?
O12 W3 O3 87.5(3) . . ?
O6 W3 O2 101.1(3) . . ?
O11 W3 O2 87.9(3) . . ?
O12 W3 O2 155.9(3) . . ?
O3 W3 O2 83.3(3) . . ?
O6 W3 K2 47.8(2) . 4_665 ?
O11 W3 K2 98.6(2) . 4_665 ?
O12 W3 K2 150.1(2) . 4_665 ?
O3 W3 K2 94.7(2) . 4_665 ?
O2 W3 K2 53.3(2) . 4_665 ?
O6 W3 K3' 54.5(3) . 2_545 ?
O11 W3 K3' 157.5(3) . 2_545 ?
O12 W3 K3' 92.3(4) . 2_545 ?
O3 W3 K3' 47.4(3) . 2_545 ?
O2 W3 K3' 97.6(5) . 2_545 ?
K2 W3 K3' 68.4(3) 4_665 2_545 ?
O19 W4 O29 105.1(3) . . ?
O19 W4 O18 102.5(3) . . ?
O29 W4 O18 94.9(3) . . ?
O19 W4 O13 101.0(3) . . ?
O29 W4 O13 89.3(3) . . ?
O18 W4 O13 154.1(3) . . ?
O19 W4 O7 97.9(3) . . ?
O29 W4 O7 156.4(3) . . ?
O18 W4 O7 85.3(3) . . ?
O13 W4 O7 80.8(3) . . ?
O19 W4 O25 168.7(3) . . ?
O29 W4 O25 84.2(2) . . ?
O18 W4 O25 82.7(2) . . ?
O13 W4 O25 72.3(2) . . ?
O7 W4 O25 72.4(2) . . ?
O19 W4 K4 51.4(2) . 2_545 ?
O29 W4 K4 156.3(2) . 2_545 ?
O18 W4 K4 88.97(19) . 2_545 ?
O13 W4 K4 97.35(19) . 2_545 ?
O7 W4 K4 47.20(19) . 2_545 ?
O25 W4 K4 119.49(15) . 2_545 ?
O20 W5 O30 104.0(3) . . ?
O20 W5 O13 101.6(3) . . ?
O30 W5 O13 91.9(3) . . ?
O20 W5 O14 100.7(3) . . ?
O30 W5 O14 90.9(3) . . ?
O13 W5 O14 156.1(3) . . ?
O20 W5 O8 99.2(3) . . ?
O30 W5 O8 156.8(3) . . ?
O13 W5 O8 83.6(3) . . ?
O14 W5 O8 84.5(3) . . ?
O20 W5 O25 171.3(3) . . ?
O30 W5 O25 83.4(2) . . ?
O13 W5 O25 73.3(2) . . ?
O14 W5 O25 83.4(2) . . ?
O8 W5 O25 73.4(2) . . ?
O20 W5 K3' 37.3(4) . 3_566 ?
O30 W5 K3' 69.2(3) . 3_566 ?
O13 W5 K3' 89.6(5) . 3_566 ?
O14 W5 K3' 113.5(5) . 3_566 ?
O8 W5 K3' 133.3(3) . 3_566 ?
O25 W5 K3' 147.3(4) . 3_566 ?
O20 W5 K1 84.0(2) . . ?
O30 W5 K1 137.4(2) . . ?
O13 W5 K1 128.0(2) . . ?
O14 W5 K1 46.70(18) . . ?
O8 W5 K1 44.78(19) . . ?
O25 W5 K1 93.58(15) . . ?
K3' W5 K1 118.6(4) 3_566 . ?
O20 W5 K3 34.7(4) . 3_566 ?
O30 W5 K3 69.7(4) . 3_566 ?
O13 W5 K3 97.4(7) . 3_566 ?
O14 W5 K3 105.8(7) . 3_566 ?
O8 W5 K3 133.5(4) . 3_566 ?
O25 W5 K3 151.4(4) . 3_566 ?
K1 W5 K3 112.6(6) . 3_566 ?
O21 W6 O31 103.7(3) . . ?
O21 W6 O15 101.0(3) . . ?
O31 W6 O15 92.6(3) . . ?
O21 W6 O14 100.7(3) . . ?
O31 W6 O14 90.8(3) . . ?
O15 W6 O14 156.5(3) . . ?
O21 W6 O9 99.2(3) . . ?
O31 W6 O9 157.1(3) . . ?
O15 W6 O9 83.5(3) . . ?
O14 W6 O9 84.4(3) . . ?
O21 W6 O26 170.9(3) . . ?
O31 W6 O26 84.1(2) . . ?
O15 W6 O26 73.7(2) . . ?
O14 W6 O26 83.6(2) . . ?
O9 W6 O26 73.2(2) . . ?
O21 W6 K5 42.2(3) . 1_455 ?
O31 W6 K5 100.4(2) . 1_455 ?
O15 W6 K5 58.9(2) . 1_455 ?
O14 W6 K5 142.82(19) . 1_455 ?
O9 W6 K5 96.81(19) . 1_455 ?
O26 W6 K5 132.49(16) . 1_455 ?
O21 W6 K1 83.9(2) . . ?
O31 W6 K1 137.9(2) . . ?
O15 W6 K1 127.1(2) . . ?
O14 W6 K1 47.26(18) . . ?
O9 W6 K1 44.23(19) . . ?
O26 W6 K1 93.41(15) . . ?
K5 W6 K1 111.50(8) 1_455 . ?
O22 W7 O32 103.4(3) . . ?
O22 W7 O16 101.9(3) . . ?
O32 W7 O16 94.6(3) . . ?
O22 W7 O15 101.1(3) . . ?
O32 W7 O15 88.3(3) . . ?
O16 W7 O15 155.3(3) . . ?
O22 W7 O10 100.0(3) . . ?
O32 W7 O10 155.9(3) . . ?
O16 W7 O10 85.9(3) . . ?
O15 W7 O10 81.7(3) . . ?
O22 W7 O26 170.0(3) . . ?
O32 W7 O26 83.8(3) . . ?
O16 W7 O26 84.1(2) . . ?
O15 W7 O26 71.9(2) . . ?
O10 W7 O26 72.3(2) . . ?
O23 W8 O33 103.8(3) . . ?
O23 W8 O16 100.8(3) . . ?
O33 W8 O16 93.7(3) . . ?
O23 W8 O17 101.4(3) . . ?
O33 W8 O17 91.4(3) . . ?
O16 W8 O17 155.3(3) . . ?
O23 W8 O11 101.0(3) . . ?
O33 W8 O11 155.1(3) . . ?
O16 W8 O11 84.0(3) . . ?
O17 W8 O11 81.3(3) . . ?
O23 W8 O27 171.8(3) . . ?
O33 W8 O27 82.7(3) . . ?
O16 W8 O27 83.7(2) . . ?
O17 W8 O27 73.0(2) . . ?
O11 W8 O27 72.4(2) . . ?
O23 W8 K3 59.3(4) . . ?
O33 W8 K3 44.5(4) . . ?
O16 W8 K3 101.4(8) . . ?
O17 W8 K3 99.1(8) . . ?
O11 W8 K3 160.1(4) . . ?
O27 W8 K3 126.9(4) . . ?
O23 W8 K3' 59.8(3) . . ?
O33 W8 K3' 44.9(3) . . ?
O16 W8 K3' 93.1(5) . . ?
O17 W8 K3' 107.3(5) . . ?
O11 W8 K3' 159.8(3) . . ?
O27 W8 K3' 127.3(2) . . ?
O23 W8 K4 36.1(3) . . ?
O33 W8 K4 114.6(2) . . ?
O16 W8 K4 66.1(2) . . ?
O17 W8 K4 132.3(2) . . ?
O11 W8 K4 87.21(19) . . ?
O27 W8 K4 145.33(15) . . ?
K3 W8 K4 77.9(5) . . ?
K3' W8 K4 73.4(3) . . ?
O24 W9 O34 105.3(3) . . ?
O24 W9 O18 100.6(3) . . ?
O34 W9 O18 94.1(3) . . ?
O24 W9 O17 100.7(3) . . ?
O34 W9 O17 91.2(3) . . ?
O18 W9 O17 155.9(3) . . ?
O24 W9 O12 96.9(3) . . ?
O34 W9 O12 157.6(3) . . ?
O18 W9 O12 84.5(3) . . ?
O17 W9 O12 81.8(3) . . ?
O24 W9 O27 169.6(3) . . ?
O34 W9 O27 84.2(3) . . ?
O18 W9 O27 82.9(2) . . ?
O17 W9 O27 74.2(2) . . ?
O12 W9 O27 73.5(2) . . ?
W1 O1 W2 150.2(3) . . ?
W1 O1 K1 105.2(3) . . ?
W2 O1 K1 102.4(2) . . ?
W2 O2 W3 152.3(4) . . ?
W2 O2 K2 103.4(3) . 4_665 ?
W3 O2 K2 95.6(2) . 4_665 ?
W1 O3 W3 153.2(3) . . ?
W1 O3 K3' 96.5(5) . 2_545 ?
W3 O3 K3' 104.3(4) . 2_545 ?
W1 O3 K3 89.8(6) . 2_545 ?
W3 O3 K3 108.7(6) . 2_545 ?
W1 O4 K5 138.6(4) . 2_545 ?
W1 O4 K3 112.5(9) . 2_545 ?
K5 O4 K3 104.7(8) 2_545 2_545 ?
W1 O4 K3' 103.7(5) . 2_545 ?
K5 O4 K3' 110.9(4) 2_545 2_545 ?
K3 O4 K3' 10.5(6) 2_545 2_545 ?
W2 O5 K4 135.2(4) . 3_565 ?
W2 O5 K2 101.7(3) . 4_665 ?
K4 O5 K2 120.8(3) 3_565 4_665 ?
W3 O6 K2 105.9(3) . 4_665 ?
W3 O6 K3' 100.1(4) . 2_545 ?
K2 O6 K3' 89.1(5) 4_665 2_545 ?
W1 O7 W4 127.0(3) . . ?
W1 O7 K4 130.2(3) . 2_545 ?
W4 O7 K4 102.8(2) . 2_545 ?
W1 O8 W5 125.3(3) . . ?
W1 O8 K1 103.1(3) . . ?
W5 O8 K1 106.6(2) . . ?
W2 O9 W6 126.0(3) . . ?
W2 O9 K1 102.0(2) . . ?
W6 O9 K1 107.0(3) . . ?
W2 O10 W7 126.7(3) . . ?
W3 O11 W8 126.3(3) . . ?
W3 O12 W9 125.0(3) . . ?
W5 O13 W4 123.9(3) . . ?
W6 O14 W5 148.0(3) . . ?
W6 O14 K1 104.7(2) . . ?
W5 O14 K1 105.4(2) . . ?
W6 O15 W7 124.6(3) . . ?
W6 O15 K5 91.2(2) . 1_455 ?
W7 O15 K5 144.1(3) . 1_455 ?
W7 O16 W8 147.7(4) . . ?
W9 O17 W8 122.6(3) . . ?
W9 O18 W4 148.8(3) . . ?
W4 O19 K1 141.4(4) . 4_666 ?
W4 O19 K4 103.1(3) . 2_545 ?
K1 O19 K4 112.7(2) 4_666 2_545 ?
W5 O20 K3' 120.8(5) . 3_566 ?
W5 O20 K3 124.8(6) . 3_566 ?
W5 O20 K2 139.0(3) . . ?
K3' O20 K2 96.4(3) 3_566 . ?
K3 O20 K2 95.1(5) 3_566 . ?
W6 O21 K5 112.9(4) . 1_455 ?
W7 O22 K2 156.8(4) . 2_455 ?
W8 O23 K4 122.9(4) . . ?
W8 O23 K5 130.4(4) . . ?
K4 O23 K5 103.0(3) . . ?
W8 O23 K3 92.8(5) . . ?
K4 O23 K3 107.9(8) . . ?
K5 O23 K3 90.1(7) . . ?
W8 O23 K3' 92.9(4) . . ?
K4 O23 K3' 100.0(5) . . ?
K5 O23 K3' 97.3(5) . . ?
P1 O25 W5 126.2(3) . . ?
P1 O25 W4 125.0(3) . . ?
W5 O25 W4 90.0(2) . . ?
P1 O25 W1 126.6(3) . . ?
W5 O25 W1 88.46(19) . . ?
W4 O25 W1 88.63(19) . . ?
P1 O26 W6 125.6(3) . . ?
P1 O26 W7 125.1(3) . . ?
W6 O26 W7 89.40(19) . . ?
P1 O27 W9 125.9(3) . . ?
P1 O27 W8 125.5(3) . . ?
W9 O27 W8 89.13(19) . . ?
P1 O28 Co2 122.1(3) . 3_566 ?
P1 O28 Co1 123.9(3) . 3_566 ?
Co2 O28 Co1 92.6(2) 3_566 3_566 ?
P1 O28 Co1 122.8(3) . . ?
Co2 O28 Co1 91.6(2) 3_566 . ?
Co1 O28 Co1 95.4(2) 3_566 . ?
W4 O29 Co1 137.9(4) . 3_566 ?
W5 O30 Co1 133.6(3) . 3_566 ?
W5 O30 Co2 125.0(3) . . ?
Co1 O30 Co2 99.1(3) 3_566 . ?
W6 O31 Co1 132.7(3) . . ?
W6 O31 Co2 125.6(3) . . ?
Co1 O31 Co2 100.0(3) . . ?
W7 O32 Co1 138.7(4) . . ?
W8 O33 Co2 138.7(4) . 3_566 ?
W8 O33 K3 108.5(6) . . ?
Co2 O33 K3 105.8(7) 3_566 . ?
W8 O33 K3' 108.6(4) . . ?
Co2 O33 K3' 109.5(4) 3_566 . ?
W9 O34 Co2 137.2(4) . 3_566 ?
O36 K1 O19 119.9(3) . 4_565 ?
O36 K1 O38 85.8(4) . . ?
O19 K1 O38 72.6(3) 4_565 . ?
O36 K1 O1 145.2(3) . . ?
O19 K1 O1 92.8(2) 4_565 . ?
O38 K1 O1 93.9(3) . . ?
O36 K1 O37 71.9(3) . . ?
O19 K1 O37 84.2(3) 4_565 . ?
O38 K1 O37 134.0(3) . . ?
O1 K1 O37 127.1(3) . . ?
O36 K1 O9 127.3(3) . . ?
O19 K1 O9 93.6(2) 4_565 . ?
O38 K1 O9 145.8(4) . . ?
O1 K1 O9 54.79(18) . . ?
O37 K1 O9 72.7(2) . . ?
O36 K1 O8 92.3(3) . . ?
O19 K1 O8 135.2(2) 4_565 . ?
O38 K1 O8 80.3(3) . . ?
O1 K1 O8 53.61(19) . . ?
O37 K1 O8 138.4(3) . . ?
O9 K1 O8 89.12(18) . . ?
O36 K1 O14 87.7(3) . . ?
O19 K1 O14 146.5(2) 4_565 . ?
O38 K1 O14 132.3(3) . . ?
O1 K1 O14 66.97(18) . . ?
O37 K1 O14 87.5(3) . . ?
O9 K1 O14 53.01(18) . . ?
O8 K1 O14 52.79(17) . . ?
O36 K1 W2 154.1(2) . . ?
O19 K1 W2 81.48(16) 4_565 . ?
O38 K1 W2 116.3(3) . . ?
O1 K1 W2 30.05(13) . . ?
O37 K1 W2 98.1(2) . . ?
O9 K1 W2 29.50(12) . . ?
O8 K1 W2 79.35(14) . . ?
O14 K1 W2 67.66(13) . . ?
O36 K1 W1 119.9(2) . . ?
O19 K1 W1 108.23(18) 4_565 . ?
O38 K1 W1 75.8(3) . . ?
O1 K1 W1 29.02(13) . . ?
O37 K1 W1 150.1(2) . . ?
O9 K1 W1 79.34(13) . . ?
O8 K1 W1 28.86(13) . . ?
O14 K1 W1 66.98(12) . . ?
W2 K1 W1 58.74(4) . . ?
O36 K1 W6 101.1(2) . . ?
O19 K1 W6 120.57(16) 4_565 . ?
O38 K1 W6 156.6(3) . . ?
O1 K1 W6 67.66(13) . . ?
O37 K1 W6 69.0(2) . . ?
O9 K1 W6 28.78(13) . . ?
O8 K1 W6 77.13(13) . . ?
O14 K1 W6 28.02(12) . . ?
W2 K1 W6 53.24(4) . . ?
W1 K1 W6 81.42(5) . . ?
O36 K1 W5 79.5(2) . . ?
O19 K1 W5 159.57(18) 4_565 . ?
O38 K1 W5 104.8(2) . . ?
O1 K1 W5 66.94(14) . . ?
O37 K1 W5 109.7(2) . . ?
O9 K1 W5 77.21(13) . . ?
O8 K1 W5 28.66(12) . . ?
O14 K1 W5 27.89(12) . . ?
W2 K1 W5 81.79(5) . . ?
W1 K1 W5 52.48(3) . . ?
W6 K1 W5 55.64(3) . . ?
O45 K2 O22 81.3(6) . 2_445 ?
O45 K2 O36 91.6(7) . . ?
O22 K2 O36 70.9(3) 2_445 . ?
O45 K2 O39 149.7(6) . . ?
O22 K2 O39 122.0(3) 2_445 . ?
O36 K2 O39 80.1(3) . . ?
O45 K2 O6 76.5(6) . 4_566 ?
O22 K2 O6 145.4(3) 2_445 4_566 ?
O36 K2 O6 135.2(3) . 4_566 ?
O39 K2 O6 89.0(3) . 4_566 ?
O45 K2 O45' 23.3(10) . . ?
O22 K2 O45' 79.8(9) 2_445 . ?
O36 K2 O45' 112.6(12) . . ?
O39 K2 O45' 158.0(10) . . ?
O6 K2 O45' 69.3(10) 4_566 . ?
O45 K2 O20 79.0(6) . . ?
O22 K2 O20 138.7(2) 2_445 . ?
O36 K2 O20 73.7(3) . . ?
O39 K2 O20 70.7(3) . . ?
O6 K2 O20 61.7(2) 4_566 . ?
O45' K2 O20 94.9(9) . . ?
O45 K2 O2 112.8(7) . 4_566 ?
O22 K2 O2 109.8(2) 2_445 4_566 ?
O36 K2 O2 155.5(3) . 4_566 ?
O39 K2 O2 79.3(2) . 4_566 ?
O6 K2 O2 57.35(19) 4_566 4_566 ?
O45' K2 O2 91.2(12) . 4_566 ?
O20 K2 O2 111.2(2) . 4_566 ?
O45 K2 O44' 68.8(8) . 4_566 ?
O22 K2 O44' 67.3(5) 2_445 4_566 ?
O36 K2 O44' 135.9(6) . 4_566 ?
O39 K2 O44' 135.2(6) . 4_566 ?
O6 K2 O44' 79.9(5) 4_566 4_566 ?
O45' K2 O44' 46.6(12) . 4_566 ?
O20 K2 O44' 134.8(6) . 4_566 ?
O2 K2 O44' 58.1(5) 4_566 4_566 ?
O45 K2 O5 145.8(6) . 4_566 ?
O22 K2 O5 76.4(2) 2_445 4_566 ?
O36 K2 O5 105.0(3) . 4_566 ?
O39 K2 O5 64.1(3) . 4_566 ?
O6 K2 O5 108.8(2) 4_566 4_566 ?
O45' K2 O5 125.2(11) . 4_566 ?
O20 K2 O5 134.0(2) . 4_566 ?
O2 K2 O5 53.61(17) 4_566 4_566 ?
O44' K2 O5 78.6(6) 4_566 4_566 ?
O45 K2 W3 93.3(6) . 4_566 ?
O22 K2 W3 132.93(19) 2_445 4_566 ?
O36 K2 W3 156.1(2) . 4_566 ?
O39 K2 W3 84.0(2) . 4_566 ?
O6 K2 W3 26.27(14) 4_566 4_566 ?
O45' K2 W3 78.0(11) . 4_566 ?
O20 K2 W3 84.36(15) . 4_566 ?
O2 K2 W3 31.07(12) 4_566 4_566 ?
O44' K2 W3 67.2(5) 4_566 4_566 ?
O5 K2 W3 83.46(14) 4_566 4_566 ?
O45 K2 W2 134.5(6) . 4_566 ?
O22 K2 W2 93.05(19) 2_445 4_566 ?
O36 K2 W2 129.3(2) . 4_566 ?
O39 K2 W2 68.3(2) . 4_566 ?
O6 K2 W2 84.16(16) 4_566 4_566 ?
O45' K2 W2 111.1(12) . 4_566 ?
O20 K2 W2 126.21(16) . 4_566 ?
O2 K2 W2 28.27(12) 4_566 4_566 ?
O44' K2 W2 67.4(5) 4_566 4_566 ?
O5 K2 W2 25.36(12) 4_566 4_566 ?
W3 K2 W2 58.34(6) 4_566 4_566 ?
O39 K3 O33 141.4(18) 3_566 . ?
O39 K3 O4 70.5(7) 3_566 2 ?
O33 K3 O4 119.8(10) . 2 ?
O39 K3 O20 75.5(7) 3_566 3_566 ?
O33 K3 O20 96.5(7) . 3_566 ?
O4 K3 O20 142.6(10) 2 3_566 ?
O39 K3 O35 85.2(12) 3_566 3_566 ?
O33 K3 O35 58.2(7) . 3_566 ?
O4 K3 O35 126.4(17) 2 3_566 ?
O20 K3 O35 64.1(6) 3_566 3_566 ?
O39 K3 O23 128.8(13) 3_566 . ?
O33 K3 O23 54.8(5) . . ?
O4 K3 O23 66.4(6) 2 . ?
O20 K3 O23 151.0(9) 3_566 . ?
O35 K3 O23 98.8(10) 3_566 . ?
O39 K3 O3 76.3(6) 3_566 2 ?
O33 K3 O3 141.7(15) . 2 ?
O4 K3 O3 55.5(5) 2 2 ?
O20 K3 O3 101.7(10) 3_566 2 ?
O35 K3 O3 159.3(10) 3_566 2 ?
O23 K3 O3 100.0(8) . 2 ?
O39 K3 O41 76.2(12) 3_566 . ?
O33 K3 O41 71.5(9) . . ?
O4 K3 O41 76.2(10) 2 . ?
O20 K3 O41 110.5(13) 3_566 . ?
O35 K3 O41 51.4(8) 3_566 . ?
O23 K3 O41 67.9(7) . . ?
O3 K3 O41 130.1(9) 2 . ?
O39 K3 O40' 131.5(13) 3_566 . ?
O33 K3 O40' 78.1(12) . . ?
O4 K3 O40' 120.8(17) 2 . ?
O20 K3 O40' 72.4(10) 3_566 . ?
O35 K3 O40' 111.2(11) 3_566 . ?
O23 K3 O40' 94.7(13) . . ?
O3 K3 O40' 75.8(13) 2 . ?
O41 K3 O40' 149.6(11) . . ?
O39 K3 W8 142.4(16) 3_566 . ?
O33 K3 W8 27.0(3) . . ?
O4 K3 W8 93.5(7) 2 . ?
O20 K3 W8 123.4(7) 3_566 . ?
O35 K3 W8 77.4(7) 3_566 . ?
O23 K3 W8 27.9(2) . . ?
O3 K3 W8 123.1(10) 2 . ?
O41 K3 W8 66.9(6) . . ?
O40' K3 W8 86.0(11) . . ?
O39 K3 W1 71.2(5) 3_566 2 ?
O33 K3 W1 134.8(8) . 2 ?
O4 K3 W1 25.0(3) 2 2 ?
O20 K3 W1 126.6(9) 3_566 2 ?
O35 K3 W1 147.9(14) 3_566 2 ?
O23 K3 W1 80.6(5) . 2 ?
O3 K3 W1 30.5(2) 2 2 ?
O41 K3 W1 100.6(8) . 2 ?
O40' K3 W1 100.7(14) . 2 ?
W8 K3 W1 108.3(6) . 2 ?
O39 K3 Co2 116.9(12) 3_566 3_566 ?
O33 K3 Co2 30.8(3) . 3_566 ?
O4 K3 Co2 141.4(13) 2 3_566 ?
O20 K3 Co2 69.4(5) 3_566 3_566 ?
O35 K3 Co2 32.5(3) 3_566 3_566 ?
O23 K3 Co2 83.8(6) . 3_566 ?
O3 K3 Co2 159.7(14) 2 3_566 ?
O41 K3 Co2 69.9(7) . 3_566 ?
O40' K3 Co2 84.1(10) . 3_566 ?
W8 K3 Co2 56.5(4) . 3_566 ?
W1 K3 Co2 164.0(8) 2 3_566 ?
O20 K3' O33 95.2(4) 3_566 . ?
O20 K3' O4 134.1(9) 3_566 2 ?
O33 K3' O4 111.9(7) . 2 ?
O20 K3' O3 108.8(5) 3_566 2 ?
O33 K3' O3 154.2(7) . 2 ?
O4 K3' O3 57.1(3) 2 2 ?
O20 K3' O39 70.5(5) 3_566 3_566 ?
O33 K3' O39 122.7(10) . 3_566 ?
O4 K3' O39 63.7(6) 2 3_566 ?
O3 K3' O39 75.7(4) 2 3_566 ?
O20 K3' O42 132.3(11) 3_566 . ?
O33 K3' O42 94.6(6) . . ?
O4 K3' O42 83.3(4) 2 . ?
O3 K3' O42 62.5(5) 2 . ?
O39 K3' O42 136.6(5) 3_566 . ?
O20 K3' O6 59.3(4) 3_566 2 ?
O33 K3' O6 141.3(8) . 2 ?
O4 K3' O6 106.6(4) 2 2 ?
O3 K3' O6 53.6(3) 2 2 ?
O39 K3' O6 78.6(4) 3_566 2 ?
O42 K3' O6 85.3(7) . 2 ?
O20 K3' O23 147.0(6) 3_566 . ?
O33 K3' O23 53.4(3) . . ?
O4 K3' O23 63.6(4) 2 . ?
O3 K3' O23 104.0(4) 2 . ?
O39 K3' O23 115.1(9) 3_566 . ?
O42 K3' O23 67.8(4) . . ?
O6 K3' O23 151.9(8) 2 . ?
O20 K3' O35 59.1(4) 3_566 3_566 ?
O33 K3' O35 52.9(4) . 3_566 ?
O4 K3' O35 109.0(10) 2 3_566 ?
O3 K3' O35 149.5(9) 2 3_566 ?
O39 K3' O35 73.9(7) 3_566 3_566 ?
O42 K3' O35 147.4(5) . 3_566 ?
O6 K3' O35 117.7(4) 2 3_566 ?
O23 K3' O35 90.2(6) . 3_566 ?
O20 K3' O40 79.2(6) 3_566 . ?
O33 K3' O40 87.7(7) . . ?
O4 K3' O40 135.6(9) 2 . ?
O3 K3' O40 87.8(8) 2 . ?
O39 K3' O40 138.0(6) 3_566 . ?
O42 K3' O40 54.7(7) . . ?
O6 K3' O40 60.9(6) 2 . ?
O23 K3' O40 106.2(8) . . ?
O35 K3' O40 114.4(5) 3_566 . ?
O20 K3' W1 128.4(5) 3_566 2 ?
O33 K3' W1 133.4(5) . 2 ?
O4 K3' W1 26.64(16) 2 2 ?
O3 K3' W1 30.64(17) 2 2 ?
O39 K3' W1 68.7(4) 3_566 2 ?
O42 K3' W1 69.4(4) . 2 ?
O6 K3' W1 82.6(3) 2 2 ?
O23 K3' W1 80.3(3) . 2 ?
O35 K3' W1 132.4(9) 3_566 2 ?
O20 K3' W8 121.6(4) 3_566 . ?
O33 K3' W8 26.45(19) . . ?
O4 K3' W8 89.4(4) 2 . ?
O3 K3' W8 129.1(5) 2 . ?
O39 K3' W8 125.9(9) 3_566 . ?
O42 K3' W8 77.9(4) . . ?
O6 K3' W8 155.4(10) 2 . ?
O23 K3' W8 27.33(16) . . ?
O35 K3' W8 72.3(4) 3_566 . ?
O40 K3' W8 94.5(7) . . ?
W1 K3' W8 107.6(4) 2 . ?
O42 K4 O5 87.2(4) . 3_565 ?
O42 K4 O23 78.2(4) . . ?
O5 K4 O23 138.8(3) 3_565 . ?
O42 K4 O43 128.2(4) . . ?
O5 K4 O43 120.3(4) 3_565 . ?
O23 K4 O43 98.4(4) . . ?
O42 K4 O7 63.9(3) . 2 ?
O5 K4 O7 114.9(2) 3_565 2 ?
O23 K4 O7 92.9(2) . 2 ?
O43 K4 O7 64.7(3) . 2 ?
O42 K4 O46 163.0(6) . . ?
O5 K4 O46 80.4(5) 3_565 . ?
O23 K4 O46 103.7(5) . . ?
O43 K4 O46 68.6(7) . . ?
O7 K4 O46 132.2(6) 2 . ?
O42 K4 O44 114.8(5) . . ?
O5 K4 O44 68.9(4) 3_565 . ?
O23 K4 O44 82.7(4) . . ?
O43 K4 O44 115.9(5) . . ?
O7 K4 O44 175.6(4) 2 . ?
O46 K4 O44 49.6(7) . . ?
O42 K4 O19 89.3(3) . 2 ?
O5 K4 O19 68.6(2) 3_565 2 ?
O23 K4 O19 147.8(2) . 2 ?
O43 K4 O19 66.3(3) . 2 ?
O7 K4 O19 55.17(18) 2 2 ?
O46 K4 O19 96.9(6) . 2 ?
O44 K4 O19 129.2(4) . 2 ?
O42 K4 O47 132.9(7) . . ?
O5 K4 O47 127.6(7) 3_565 . ?
O23 K4 O47 54.8(6) . . ?
O43 K4 O47 65.5(6) . . ?
O7 K4 O47 113.3(7) 2 . ?
O46 K4 O47 51.8(8) . . ?
O44 K4 O47 64.1(7) . . ?
O19 K4 O47 129.6(5) 2 . ?
O42 K4 W4 73.7(3) . 2 ?
O5 K4 W4 88.27(17) 3_565 2 ?
O23 K4 W4 122.89(18) . 2 ?
O43 K4 W4 65.2(3) . 2 ?
O7 K4 W4 30.01(12) 2 2 ?
O46 K4 W4 117.2(6) . 2 ?
O44 K4 W4 154.4(3) . 2 ?
O19 K4 W4 25.47(13) 2 2 ?
O47 K4 W4 129.2(6) . 2 ?
O42 K4 W8 76.2(3) . . ?
O5 K4 W8 118.08(19) 3_565 . ?
O23 K4 W8 21.01(15) . . ?
O43 K4 W8 116.4(3) . . ?
O7 K4 W8 109.87(16) 2 . ?
O46 K4 W8 99.3(5) . . ?
O44 K4 W8 65.8(3) . . ?
O19 K4 W8 163.29(18) 2 . ?
O47 K4 W8 60.3(5) . . ?
W4 K4 W8 138.57(10) 2 . ?
O42 K4 K5 97.3(4) . . ?
O5 K4 K5 173.49(19) 3_565 . ?
O23 K4 K5 38.85(17) . . ?
O43 K4 K5 60.2(3) . . ?
O7 K4 K5 71.45(15) 2 . ?
O46 K4 K5 94.2(5) . . ?
O44 K4 K5 104.9(4) . . ?
O19 K4 K5 116.00(18) 2 . ?
O47 K4 K5 46.1(7) . . ?
W4 K4 K5 97.49(10) 2 . ?
W8 K4 K5 58.95(8) . . ?
O4 K5 O45 83.7(6) 2 2 ?
O4 K5 O21 138.2(3) 2 1_655 ?
O45 K5 O21 129.2(6) 2 1_655 ?
O4 K5 O38 71.1(3) 2 2 ?
O45 K5 O38 66.2(7) 2 2 ?
O21 K5 O38 97.0(3) 1_655 2 ?
O4 K5 O45' 104.4(10) 2 2 ?
O45 K5 O45' 24.1(10) 2 2 ?
O21 K5 O45' 114.6(10) 1_655 2 ?
O38 K5 O45' 85.1(11) 2 2 ?
O4 K5 O23 71.7(2) 2 . ?
O45 K5 O23 123.1(6) 2 . ?
O21 K5 O23 101.0(2) 1_655 . ?
O38 K5 O23 140.0(4) 2 . ?
O45' K5 O23 118.1(10) 2 . ?
O4 K5 O41 79.1(3) 2 . ?
O45 K5 O41 150.8(7) 2 . ?
O21 K5 O41 59.8(2) 1_655 . ?
O38 K5 O41 85.8(4) 2 . ?
O45' K5 O41 168.6(10) 2 . ?
O23 K5 O41 73.3(2) . . ?
O4 K5 O46 150.4(5) 2 3_665 ?
O45 K5 O46 75.6(8) 2 3_665 ?
O21 K5 O46 71.0(5) 1_655 3_665 ?
O38 K5 O46 117.5(6) 2 3_665 ?
O45' K5 O46 51.9(12) 2 3_665 ?
O23 K5 O46 102.1(6) . 3_665 ?
O41 K5 O46 127.9(6) . 3_665 ?
O4 K5 O47 113.2(6) 2 . ?
O45 K5 O47 92.5(8) 2 . ?
O21 K5 O47 92.7(6) 1_655 . ?
O38 K5 O47 158.2(6) 2 . ?
O45' K5 O47 73.1(12) 2 . ?
O23 K5 O47 55.6(5) . . ?
O41 K5 O47 115.9(6) . . ?
O46 K5 O47 48.1(7) 3_665 . ?
O4 K5 O15 131.7(2) 2 1_655 ?
O45 K5 O15 76.5(6) 2 1_655 ?
O21 K5 O15 54.6(2) 1_655 1_655 ?
O38 K5 O15 60.6(3) 2 1_655 ?
O45' K5 O15 71.8(9) 2 1_655 ?
O23 K5 O15 153.9(2) . 1_655 ?
O41 K5 O15 97.7(2) . 1_655 ?
O46 K5 O15 63.6(5) 3_665 1_655 ?
O47 K5 O15 111.3(6) . 1_655 ?
O4 K5 W6 141.4(2) 2 1_655 ?
O45 K5 W6 105.7(6) 2 1_655 ?
O21 K5 W6 24.88(15) 1_655 1_655 ?
O38 K5 W6 78.7(2) 2 1_655 ?
O45' K5 W6 96.2(9) 2 1_655 ?
O23 K5 W6 125.63(19) . 1_655 ?
O41 K5 W6 75.18(18) . 1_655 ?
O46 K5 W6 66.2(5) 3_665 1_655 ?
O47 K5 W6 103.8(6) . 1_655 ?
O15 K5 W6 29.83(12) 1_655 1_655 ?
O4 K5 W1 15.92(15) 2 2 ?
O45 K5 W1 68.6(6) 2 2 ?
O21 K5 W1 153.2(2) 1_655 2 ?
O38 K5 W1 70.5(2) 2 2 ?
O45' K5 W1 88.5(10) 2 2 ?
O23 K5 W1 77.70(17) . 2 ?
O41 K5 W1 94.99(19) . 2 ?
O46 K5 W1 135.7(5) 3_665 2 ?
O47 K5 W1 107.6(6) . 2 ?
O15 K5 W1 128.09(17) 1_655 2 ?
W6 K5 W1 148.25(13) 1_655 2 ?
Co2 O35 K3 96.7(7) . 3_566 ?
Co2 O35 K3' 91.0(5) . 3_566 ?
K3 O35 K3' 7.2(6) 3_566 3_566 ?
K2 O36 K1 117.3(3) . . ?
K1 O38 K5 130.7(4) . 2_545 ?
K3 O39 K2 101.7(9) 3_566 . ?
K3 O39 K3' 8.6(7) 3_566 3_566 ?
K2 O39 K3' 94.8(5) . 3_566 ?
K5 O41 K3 85.1(5) . . ?
K4 O42 K3' 108.4(6) . . ?
O44' O44 K4 174(4) . . ?
O44 O44' K2 170(4) . 4_665 ?
K2 O45 K5 152.5(11) . 2_545 ?
K5 O45' K2 129(2) 2_545 . ?
K4 O46 K5 174.2(10) . 3_665 ?
K5 O47 K4 86.1(7) . . ?

_refine_diff_density_max         3.368
_refine_diff_density_min         -3.924
_refine_diff_density_rms         0.455

